
系統識別號 
U00262906201723162600 
論文名稱(中文) 
晶粒尺寸對奈米結構316LVM不銹鋼塑性變形行為及微觀結構特性之效應分析 
論文名稱(英文) 
The Influence of Grain Size on the Plastic Deformation and Microstructure of Nanostructured 316LVM Stainless Steel 
校院名稱 
成功大學 
系所名稱(中) 
機械工程學系 
系所名稱(英) 
Department of Mechanical Engineering 
學年度 
105 
學期 
2 
出版年 
106 
研究生(中文) 
呂名祺 
研究生(英文) 
MingChi Lu 
學號 
N16044682 
學位類別 
碩士 
語文別 
中文 
論文頁數 
105頁 
口試委員 
指導教授李偉賢 口試委員王俊志 口試委員黃永茂

中文關鍵字 
霍普金森桿
316LVM不銹鋼
晶粒大小
高應變速率
差排密度

英文關鍵字 
Hopkinson bar
high strain rate
316LVM stainless steel
HallPetch
dislocation density

學科別分類 

中文摘要 
本篇論文主要使用霍普金森試驗機在室溫(25℃)下對不同晶粒尺寸的316LVM不銹鋼進行撞擊試驗，並觀測其機械性質及微觀結構的變化。本次實驗，透過退火處理後得到兩不同大小之晶粒尺寸，分別為32μm和64μm，所採用之應變速率分別為3000s1、5000s1和7000s1，再透過所得到之數據以及微觀結構(OM、TEM)進行分析，藉此了解相同的材料，不同的晶粒尺寸以及應變速率對材料塑變行為及微觀結構之影響。最後利用ZerilliArmstronge構成方程式進行模擬，以描述316LVM不銹鋼在各應變速率、晶粒大小及塑流應力之關係，以方便未來在作為工程模擬分析之用途。
實驗結果指出，晶粒尺寸大小的不同對316LVM不銹鋼的機械性質影響相當明顯，為描述晶粒大小與塑流應力之關係，引用HallPatch方程式印證晶粒愈小則塑流應力愈大的結果。而隨著材料變形的應變速率提升，其塑流應力值、加工硬化率、應變速率敏感性係數皆會跟著上升，而熱活化體積則會隨著應變速率上升而下降。
在微觀方面，透過穿透式電子顯微鏡的觀測，材料在遭受撞擊後差排會糾結在一起，且差排密度會隨著應變速率上升而增加，而差排密度與塑流應力之關係可由BaileyHirsch type關係式來描述，此外當隨著應變速率的上升，甚至可觀測到差排環以及機械雙晶的產生。

英文摘要 
In this study, 316LVM stainless steel was examined under different strain rates and grain sizes by using splitHopkinson pressure bar to investigate its dynamic deformation behaviors and microstructure characteristics. Impact tests were performed under different strain rates ranging from 3×103 s1 to 7×103 s1 and different grain sizes of 32μm and 64μm at room temperature.
The results reveal that the mechanical properties are greatly affected by strain rates and grain sizes and the HallPetch equation can describe the relationship between flow stress and grain size. It is found that flow stress, work hardening rate and strain rate sensitivity all increase, but the thermal activation volume decreases with the increasing strain rate. However, at a constant strain rate, flow stress, work hardening rate and strain rate sensitivity decrease but the thermal activation volume increases with increasing grain size. Finally, the modified ZerilliArmstrong model, which combine ZerilliArmstrong model with HallPetch equation, is used to describe the deformation behavior of 316LVM stainless steel under the considered strain rate and grain size.
Transmission electron microscope(TEM) observations show that the dislocation density increases with increasing strain rate but decreases with increasing grain size. The relationship between the dislocation density and the stress can be expressed by using the BaileyHirsch equation. Furthermore, dislocation loops and mechanical twins are found at high strain rate.

論文目次 
中文摘要 I
ABSTRACT II
致謝 IX
總目錄 X
表目錄 XIII
圖目錄 XIV
符號說明 XIX
第一章 前言 1
第二章 理論與文獻回顧 4
21 不銹鋼之介紹 4
211 肥粒鐵系 4
212 麻田散鐵系 4
213 沃斯田鐵系 5
214 雙相系 5
215 析出硬化系 6
22 塑性變形之機械測試類別 6
221 靜態或極低之應變速率（108＜ε ̇＜105 s1）： 6
222 低速之應變速率（105＜ε ̇＜100 s1）： 7
223 中速之應變速率（100＜ε ̇＜102 s1）： 7
224 高速之應變速率（102＜ε ̇＜104 s1）： 7
225 極高速之應變速率（104＜ε ̇＜107 s1）： 7
23 一維波傳理論 8
24 霍普金森撞擊試驗機之原理 10
25 材料塑變行為特性 12
251 恆溫機制 13
252 熱活化機制 13
253 差排黏滯機制 15
26 構成方程式 16
261 Ludwik model[2224] 16
262 Sokolosky& Malvern model[24] 16
263 ZerilliArmstrong model[25, 26] 17
264 JohnsonCook model[2730] 17
第三章 實驗方法及步驟 26
31 實驗流程 26
32 實驗儀器與設備 26
321 霍普金森撞擊試驗機 26
322 研磨拋光機 28
323 慢速切割機 28
324 雙噴射式電解拋光機 28
325 CNC放電加工線切割機 29
326 光學顯微鏡 29
327 穿透式電子顯微鏡 29
33 實驗步驟 30
331 實驗試件製備 30
332 改變晶粒尺寸 30
333 動態衝擊試驗 30
334 試件金相之觀察(OM) 31
335 穿透式電子顯微鏡(TEM)試片製備 31
第四章 實驗結果與討論 34
41 應力應變曲線 34
42 應力晶粒關係 34
43 加工硬化 35
44 應變速率敏感性係數 36
45 熱活化體積 37
46 理論溫升量 39
47 材料構成方程式 39
48 光學顯微鏡金相組織觀察(OM) 40
49 穿透式電子顯微鏡(TEM)結構觀察 41
第五章 結論 96
參考文獻 98

參考文獻 
[1] M. A. Meyers, Dynamic behavior of materials: John wiley & sons, 1994.
[2] H. Kolsky, "An investigation of the mechanical properties of materials at very high rates of loading," Proceedings of the Physical Society. Section B, vol. 62, p. 676, 1949.
[3] B. Butcher and C. Karnes, "Strain‐Rate Effects in Metals," Journal of Applied Physics, vol. 37, pp. 402411, 1966.
[4] F. E. Hauser, "Techniques for measuring stressstrain relations at high strain rates," Experimental Mechanics, vol. 6, pp. 395402, 1966.
[5] D. Steinberg, S. Cochran, and M. Guinan, "A constitutive model for metals applicable at high‐strain rate," Journal of Applied Physics, vol. 51, pp. 14981504, 1980.
[6] S. Barriuso, J. Chao, J. A. Jiménez, S. García, and J. L. GonzálezCarrasco, "Fatigue behavior of Ti6Al4V and 316 LVM blasted with ceramic particles of interest for medical devices," Journal of the mechanical behavior of biomedical materials, vol. 30, pp. 3040, 2014.
[7] J. S. Jensen, "Mechanical strength of sliding screwplate hip implants: a biomechanical study of unstable trochanteric fractures. VI," Acta Orthopaedica Scandinavica, vol. 51, pp. 625631, 1980.
[8] M. J. Desroches, N. Chaudhary, and S. Omanovic, "PMIRRAS investigation of the interaction of serum albumin and fibrinogen with a biomedicalgrade stainless steel 316LVM surface," Biomacromolecules, vol. 8, pp. 28362844, 2007.
[9] A. Shahryari, W. Kamal, and S. Omanovic, "The effect of surface roughness on the efficiency of the cyclic potentiodynamic passivation (CPP) method in the improvement of general and pitting corrosion resistance of 316LVM stainless steel," Materials Letters, vol. 62, pp. 39063909, 2008.
[10] U. S. Lindholm, "High strain rate tests," Measurement of mechanical properties, vol. 5, pp. 199271, 1971.
[11] U. Lindholm and L. Yeakley, "High strainrate testing: tension and compression," Experimental Mechanics, vol. 8, pp. 19, 1968.
[12] J. Achenbach, Wave propagation in elastic solids vol. 16: Elsevier, 2012.
[13] B. Dodd, Adiabatic shear localization: occurrence, theories, and applications: Pergamon Press, 1992.
[14] W.S. Lee and C.F. Lin, "Plastic deformation and fracture behaviour of Ti–6Al–4V alloy loaded with high strain rate under various temperatures," Materials Science and Engineering: A, vol. 241, pp. 4859, 1998.
[15] A. Kumar, F. Hauser, and J. Dorn, "Viscous drag on dislocations in aluminum at high strain rates," Acta Metallurgica, vol. 16, pp. 11891197, 1968.
[16] J. Campbell and W. Ferguson, "The temperature and strainrate dependence of the shear strength of mild steel," Philosophical Magazine, vol. 21, pp. 6382, 1970.
[17] R. Broudy, "Dislocations and Mechanical Properties of Crystals," Journal of the American Chemical Society, vol. 80, pp. 50095010, 1958.
[18] H. Conrad, "Thermally activated deformation of metals," JOM, vol. 16, pp. 582588, 1964.
[19] W. Ferguson, A. Kumar, and J. Dorn, "Dislocation damping in aluminum at high strain rates," Journal of Applied Physics, vol. 38, pp. 18631869, 1967.
[20] J. Campbell and A. Dowling, "The behaviour of materials subjected to dynamic incremental shear loading," Journal of the Mechanics and Physics of Solids, vol. 18, pp. 4363, 1970.
[21] J. Campbell, "Dynamic plasticity: macroscopic and microscopic aspects," Materials Science and Engineering, vol. 12, pp. 321, 1973.
[22] P. Ludwik, "Elemente der Technologischen Mechanik Julius Springer," Berlin, Germany, 1909.
[23] Z. Gronostajski, "The constitutive equations for FEM analysis," Journal of Materials Processing Technology, vol. 106, pp. 4044, 2000.
[24] Y. Bai and B. Dodd, "Adiabatic Shear Localization: Occurrence, Theories and Applications, 1992," ed: Pergamon Press, Oxford.
[25] F. J. Zerilli and R. W. Armstrong, "The effect of dislocation drag on the stressstrain behavior of FCC metals," Acta Metallurgica et Materialia, vol. 40, pp. 18031808, 1992.
[26] R. Liang and A. S. Khan, "A critical review of experimental results and constitutive models for BCC and FCC metals over a wide range of strain rates and temperatures," International Journal of Plasticity, vol. 15, pp. 963980, 1999.
[27] D. Umbrello, R. M’saoubi, and J. Outeiro, "The influence of Johnson–Cook material constants on finite element simulation of machining of AISI 316L steel," International Journal of Machine Tools and Manufacture, vol. 47, pp. 462470, 2007.
[28] L. Meyer, N. Herzig, T. Halle, F. Hahn, L. Krueger, and K. Staudhammer, "A basic approach for strain rate dependent energy conversion including heat transfer effects: An experimental and numerical study," Journal of materials processing technology, vol. 182, pp. 319326, 2007.
[29] G. R. Johnson and W. H. Cook, "A constitutive model and data for metals subjected to large strains, high strain rates and high temperatures," in Proceedings of the 7th International Symposium on Ballistics, 1983, pp. 541547.
[30] U. Andrade, M. Meyers, and A. Chokshi, "Constitutive description of workand shockhardened copper," Scripta metallurgica et materialia, vol. 30, pp. 933938, 1994.
[31] D. Klahn, A. Mukherjee, and J. Dorn, "STRAINRATE EFFECTS," California Univ., Berkeley. Lawrence Radiation Lab.1970.
[32] A. T. Krawczynska, M. Lewandowska, and K. J. Kurzydłowski, "Recrystallization in nanostructured austenitic stainless steel," in Materials Science Forum, 2008, pp. 966970.
[33] A. T. Krawczynska, M. Lewandowska, and K. J. Kurzydłowski, "Nanostructure formation in austenitic stainless steel," in Solid State Phenomena, 2008, pp. 173178.
[34] Y. Huang, A. Pequegnat, J. Feng, M. Khan, and Y. Zhou, "Resistance microwelding of crossed Pt–10Ir and 316 LVM stainless steel wires," Science and Technology of Welding and Joining, vol. 16, pp. 648656, 2011.
[35] M. Talha, C. Behera, S. Kumar, O. Pal, G. Singh, and O. Sinha, "Long term and electrochemical corrosion investigation of cold worked AISI 316L and 316LVM stainless steels in simulated body fluid," RSC Advances, vol. 4, pp. 1334013349, 2014.
[36] B. Weiss and R. Stickler, "Phase instabilities during high temperature exposure of 316 austenitic stainless steel," Metallurgical and Materials Transactions B, vol. 3, pp. 851866, 1972.
[37] R. W. Armstrong, "Material grain size and crack size influences on cleavage fracturing," Philosophical Transactions of the Royal Society of London A: Mathematical, Physical and Engineering Sciences, vol. 373, p. 20140124, 2015.
[38] A. Chokshi, A. Rosen, J. Karch, and H. Gleiter, "On the validity of the HallPetch relationship in nanocrystalline materials," Scripta Metallurgica, vol. 23, pp. 16791683, 1989.
[39] C. Huang, W. Hu, G. Yang, Z. Zhang, S. Wu, Q. Wang, et al., "The effect of stacking fault energy on equilibrium grain size and tensile properties of nanostructured copper and copper–aluminum alloys processed by equal channel angular pressing," Materials Science and Engineering: A, vol. 556, pp. 638647, 2012.
[40] S. Esmaeili, L. Cheng, A. Deschamps, D. Lloyd, and W. Poole, "The deformation behaviour of AA6111 as a function of temperature and precipitation state," Materials Science and Engineering: A, vol. 319, pp. 461465, 2001.
[41] B. Viguier, "Dislocation densities and strain hardening rate in some intermetallic compounds," Materials Science and Engineering: A, vol. 349, pp. 132135, 2003.
[42] D. Chu and J. Morris, "The influence of microstructure on work hardening in aluminum," Acta materialia, vol. 44, pp. 25992610, 1996.
[43] L. Shi and D. Northwood, "The mechanical behavior of an AISI type 310 stainless steel," Acta metallurgica et materialia, vol. 43, pp. 453460, 1995.
[44] E. Frutos, R. MartínezMorillas, J. L. GonzálezCarrasco, and N. Vilaboa, "Nanomechanical properties of novel intermetallic coatings developed on austenitic stainless steels by siliconisation in liquid phase," Intermetallics, vol. 19, pp. 260266, 2011.
[45] W.S. Lee and C.Y. Liu, "Comparison of dynamic compressive flow behavior of mild and medium steels over wide temperature range," Metallurgical and materials Transactions A, vol. 36, pp. 31753186, 2005.
[46] M. Talha, C. Behera, and O. Sinha, "Invitro long term and electrochemical corrosion resistance of cold deformed nitrogen containing austenitic stainless steels in simulated body fluid," Materials Science and Engineering: C, vol. 40, pp. 455466, 2014.
[47] H. Garbacz, M. Lewandowska, W. Pachla, and K. J. Kurzydłowski, "Structural and mechanical properties of nanocrystalline titanium and 316LVM steel processed by hydrostatic extrusion," Journal of microscopy, vol. 223, pp. 272274, 2006.
[48] N. Mottu, M. Vayer, and R. Erre, "Xe and Mo ion implantation on austenitic stainless steel: structural modification," Surface and Coatings Technology, vol. 183, pp. 165173, 2004.
[49] T. Roland, D. Retraint, K. Lu, and J. Lu, "Fatigue life improvement through surface nanostructuring of stainless steel by means of surface mechanical attrition treatment," Scripta Materialia, vol. 54, pp. 19491954, 2006.
[50] H. Zhang, Z. Hei, G. Liu, J. Lu, and K. Lu, "Formation of nanostructured surface layer on AISI 304 stainless steel by means of surface mechanical attrition treatment," Acta materialia, vol. 51, pp. 18711881, 2003.
[51] X. An, Q. Lin, S. Qu, G. Yang, S. Wu, and Z.F. Zhang, "Influence of stackingfault energy on the accommodation of severe shear strain in CuAl alloys during equalchannel angular pressing," Journal of materials research, vol. 24, pp. 36363646, 2009.
[52] F. Yan, G. Liu, N. Tao, and K. Lu, "Strength and ductility of 316L austenitic stainless steel strengthened by nanoscale twin bundles," Acta Materialia, vol. 60, pp. 10591071, 2012.
[53] H. Wang, K. Wang, Z. Liu, Y. Wang, G. Wu, and X. Duan, "TEM characterization of twinning in Co39Ni33Al28 alloy," Materials transactions, vol. 48, pp. 21392142, 2007.
[54] R. Ham, "The determination of dislocation densities in thin films," Philosophical Magazine, vol. 6, pp. 11831184, 1961.
[55] Sandvik, "DatasheetSandvikBioline316LVM."

論文全文使用權限 
同意授權校內瀏覽/列印電子全文服務，於20170705起公開。同意授權校外瀏覽/列印電子全文服務，於20170705起公開。 


